Peroxymonosulfate enhanced photocatalytic degradation of organic dye by metal-free TpTt-COF under visible light irradiation

Recently, the activation of persulfate (PDS) by non-metallic photocatalysts under visible light has attracted significant interest in applications in environmental remediation. This study presents a pioneering investigation into the combined application of the TpTt-COF and PMS for visible light degradation of organic dyes. Synthesized orange TpTt-COF monomers exhibit exceptional crystallinity, a 2D structure, and notable stability in harsh conditions. The broad visible light absorption around a wavelength of 708 nm. The TpTt-COF emerges as a promising candidate for photocatalytic dye degradation. The study addresses high charge recombination in the TpTt-COF, highlighting the crucial role of its electron donor and acceptor for the PMS activation. Comparative analyses against traditional photocatalytic materials, such as the metal-free carbon-based material g-C3N4 and transition metal-containing TiO2, demonstrate TpTt-COF's superior performance, generating diverse free radicals. In simulated experiments, the TpTt-COF's degradation rate surpasses PMS-combined g-C3N4 by 13.9 times. and 1.6 times higher than the TpTt-COF alone. Remarkably, the TpTt-COF maintains high activity under harsh environments. Investigations into the degradation mechanism and the TpTt-COF's reusability reveal its efficiency and stability. Under visible light, TpTt-COF facilitates efficient electron–hole separation. Combining the TpTt-COF with PMS produces various radicals, ensuring effective separation and a synergistic effect. Radical quenching experiments confirm the pivotal role of O2-· radicals, while ·OH and SO4-· radicals intensify the degradation. After five cycles, TpTt-COF maintains an impressive 83.2% degradation efficiency. This study introduces an efficient photocatalytic system mediated by PMS and valuable insights into governing mechanisms for organic pollutant degradation in water environments.

www.nature.com/scientificreports/methods, AOPs are considered one of the most promising technologies for the complete degradation of various dyes 9 .This technique employs highly effective oxidants for directly breaking down pollutants or utilizing the formation of oxidant-induced radicals to facilitate the process of decomposition 10 .The approach shows considerable potential for breaking down organic matter by generating highly effective and responsive reactive oxidizing species (ROS), such as hydroxyl radicals, superoxide radicals, singlet oxygen, and others.Various oxides, such as hydrogen peroxide (H 2 O 2 ), sulfate (SO 4 ), and peracetic acid (CH 3 CO 3 H), are activated through different mechanisms to produce ROSs via a sequence of radical chain reactions for the breakdown of pollutants.The resulting ROSs engage in redox reactions with organic matter, ultimately converting it into simple carbon dioxide and water.The sulfate radicals formed by the activation of PMS exhibit higher oxidation potential (2.50-3.10V) and a longer half-life of 30-40 μs (Eo = 1.90-2.70V vs. NHE, with a half-life of 20 ns) compared to •OH radicals generated by other AOPs additives.Additionally, they possess characteristics such as high selectivity, environmental friendliness, convenient transport, and low cost.Moreover, the activation of various peroxydisulfates by transition metal ions is a gentle process that does not require additional energy.For Example, Xiao et al. 11 synthesized Fe-MOF for catalytic activating PMS for the rapid degradation of methylene blue.Although transition metal-activated PMS produces highly oxidizing sulfate free radicals (SO 4 −• ) with strong degradation capacity, the metal ions are difficult to recover from high to low valence state, limiting the overall degradation capacity in PMS systems.
Photocatalysis is an efficient and environmentally friendly technology that converts solar energy into chemical activity 12 .Photocatalytic materials including transition metal sulfides 13 and oxides 14 , biomass-derived carbon 15 , and others.These materials absorb light energy, initiating the transition of electrons within the catalyst from the ground state to an excited state, resulting in the formation of electron-hole pairs.Subsequently, the interaction of electrons and holes with oxygen or water generates reactive oxygen radicals, such as •OH and •O 2− .These radicals then engage in mutual interactions with pollutants, facilitating their adsorption onto the catalyst surface and ultimately contributing to the degradation of pollutants.Additionally, photocatalysis can be combined with SR-AOPs to oxidize organic contaminants.Numerous studies demonstrated that, under visible light irradiation, photocatalysts excited electrons and holes to react with PMS, generating SO 4 -• and SO 5 -• free radicals.These radicals can attack organic pollutants, breaking them down into smaller fragments.For example, Zhang et al. 9 utilized an iron-based MOF (MIL-88A) to activate PMS for the visible light catalytic degradation of tetracycline.The Fe-MOF activated PS generated •OH, O 2 −• , SO 4 −• , S 2 O 8 −• , and other free radicals that were responsible for completely degrading tetracycline after 80 min of visible light illumination.However, these materials often suffer from rapid charge recombination, poor light utilization, and low catalytic efficiency.Therefore, Liao et al. 16 successfully synthesized rod-like MIL-88B-Fe mixed with g-C 3 N 4 .The presence of the heterojunction can effectively reduce the electron and hole recombination, demonstrating excellent photocatalytic performance with remarkable stability.It activated PMS and catalytic degradation of low-concentration RhB in about 1 h while maintaining good cyclic performance.Nevertheless, these catalysts can inevitably release metal ions during the reaction process and cause secondary pollution in water.
Photocatalytic of metal-free organic polymer driven by visible light is considered a promising method for PMS activation due to its stability, mild reaction conditions, good solar energy utilization, and high efficiency 22 .However, due to ballistic electron scattering, carbon-based catalyst materials, such as graphene, g-C3N4, and carbon nanotubes, exhibit high electrical conductivity.Hence, they suffer from poor charge separation with a high recombination rate 23,24 .To tackle this issue, doping or introducing surface defects are typically employed 25 .However, an excess of defects can hinder charge separation and result in a high density of structural defects.Furthermore, adjusting the electronic structure of these materials is also limited 26 due to the rigidity and chemical inertness of the carbon chemicals.
A covalent organic framework (COF) is an emerging material with a controllable crystal structure formed by stable periodic aromatic units through covalent bonds 27 .Two-dimensional COFs have excellent photocatalytic ability because of their extended Sp 2 hybridized orbit structure, which can promote charge carrier transport 28 .More importantly, the presence of electron donors and acceptors in the same COF is essential for stabilizing the photoexcited electrons and holes readily used for redox reaction to activate PMS.Recently, Yang et al. 29 found that COF-PRD synthesized from Tp and pyridine can photocatalytically activate PMS to degrade bisphenol A (BPA).TpTt-COF is a novel covalent organic framework material with a broad spectral response and effective light absorption in the visible range.It is synthesized through the Schiff base polymerization of Tp (phloroglucinol, containing -CHO groups) and Tt (melamine, containing -NH 2 groups).Bhadra et al. 30 synthesized TpTt-COF with a wide range of substrate scope for visible light excitation.In the presence of blue LED, TpTt-COFs were excited from the ground state to the singlet state, resulting in a more energy-stable trilinear state and interacting with trans-stilbene to form the excited states.This energy transfer aids trans-stilbene to convert to cis-stilbene through a di-radical intermediate.Feng et al. 31 demonstrated that TpTt-COF is stable and versatile in oxidative coupling of amine, such as Aniline, to air driven by visible light.Furthermore, TpTt-COF is highly stable 32 and can be easily recovered from the catalytic system, enabling efficient reuse.Unlike materials such as graphene, TpTt's electronic structure can be modified by introducing auxiliary functional groups 33,34 .Hence, their photocatalytic potential can be chemically optimized.
This study marks a pioneering exploration of the combined application of TpTt-COF and PMS for the visible light degradation of organic dyes.The synthesized orange TpTt-COF exhibits superior crystallinity compared to some other COFs 35 and shows broad visible light absorption at a wavelength of 708 nm.Additionally, it demonstrates outstanding thermal stability, reaching up to 200 °C.This TpTt-COF demonstrates robust stability in acidic and alkaline water environments 36 .The creative combination with PMS makes it applicable in the field of photodegradation of organic dyes.Compared to popular transition metal photocatalysts such as Fe-MOF 37 , the

Characterization
The crystal structures were identified by Powder X-ray diffraction (PXRD, Rigaku Smartlab) with Cu Kα (1.5418 Å) radiation over the 2θ range of 5 °-40 ° and at a scanning step of 0.02 °.The morphologies of the samples were observed by a scanning electron microscope (SEM, Hitachi SU8010).Fourier transform infrared (FTIR) spectra were collected from KBr pellets on a Spectrum One FTIR spectrophotometer (Perkin-Elmer, USA) from 4000 to 500 cm −1 at a resolution of 2 cm −1 .The thermal stability was investigated by a TG-DTG 6300 thermogravimetric analyzer (EXSTAR, Japan) from room temperature to 800 ℃ at a heating rate of 10 °C/min in N 2 flow.The band gap was obtained by UV-vis diffuse reflectance spectroscopy (UV-vis DRS, Shimadzu, Japan), collected from a dry-pressed disc sample on a PerkinElmer Lambda 650S spectrophotometer with BaSO 4 as the reference.The specific surface area was determined by the Brunauer-Emmett-Teller (BET) method, and the pore size distribution was analyzed by the Barrett-Joyner-Halenda (BJH) model.The dye concentrations were monitored by a UV-vis spectrometer (752 N, INESA, Shanghai).The elemental valence structures were analyzed by X-ray photoelectron spectroscopy (XPS, ESCALAB 250Xi, Thermo Fisher Scientific, USA).The C1s peak at 284.8 eV was used to calibrate binding energies.The photoelectrochemical current and electrochemical impedance spectroscopy measurements were conducted using an electrochemical workstation (CHI760E, Shanghai Chenhua, China).

Analytic method for determining dyes concentrations
The Methyl Orange (MO), Rhodamine B (RhB), and Methylene Blue (MB) solutions were sampled by transferring a small volume of the solution and centrifuging to remove TpTt solid.Their concentrations were analyzed by a UV-vis spectrophotometer at the peak absorption wavelengths of 463 nm, 554 nm, and 664 nm, respectively.

Photocatalytic experiments
The photocatalytic activity of the TpTt-COF was assessed by degrading different dyes (RhB, MO, and MB) under simulated visible light irradiation with PMS.A Xenon arc lamp (CHF-XM-500 W, Perfectlight, China) equipped with a UV cutoff filter (λ ≥ 400 nm) was used as the excitation source.An optical power meter (FZ400, NBeT, China) was used to ensure the optical density of 100 mW/cm 2 , corresponding to the solar energy on Earth.Based on previous research 39,40 and incorporating the insights from Figs. 5d, 6c, d, improvements were made to the method of photocatalytic degradation of organic dyes.5 mg photocatalyst powder was uniformly dispersed in 110 mL dye aqueous solution with an initial dye concentration of 10 mg/L at pH 3. To reach the adsorption-desorption equilibrium of the dyes, the mixture was stirred in the dark for 30 min before adding 25 mg of PMS and starting the photoexcitation.The processed dye solution of 4 mL was collected within the designated time interval, followed by centrifuging before measuring the concentrations.Each measurement was performed three times.

Electrochemistry measurements
Electrochemical analysis was performed using a conventional three-electrode system.Generally, catalyst-coated ITO glass (1 cm × 2 cm × 1.1 mm) was used as the working electrode.An Ag/AgCl electrode was used as the reference electrode, and a platinum foil was used as the counter electrode.The ITO substrate was ultrasonically cleaned in deionized water, acetone, and ethanol for 1 h each and then naturally dried.10 mg catalyst powder was mixed with 1 mL ethanol and 35 μL adhesive (Nafion perfluorinated resin).The resulting liquid was added dropwise on the dried ITO glass 3 times with each drop volume of 30 μL.After the glass was naturally air-dried, the electrode was immersed in the electrochemical cell, containing 20 mL Na 2 SO 4 solution (0.2 M) as the electrolyte.Transient photocurrent and electrochemical impedance spectroscopy measurements were conducted under illumination, while Mott-Schottky analysis was performed in the dark.The photoelectrochemical measurements were carried out using a CHI760E workstation (Shanghai Chenhua Instrument) illuminated by a 300 W xenon lamp (CELHXF300) equipped with a UV cutoff filter (λ ≥ 400 nm).Illumination power was calibrated to be 100 mW/cm 2 using a FZ400 optical power meter.

Characterization
The crystal structure of TpTt-COF was investigated using PXRD, as shown in Fig. 2a.Distinct peaks at 9.7° and 27.4° were observed, attributed to the diffraction from the (100) and (002) planes, respectively.The presence of these peaks signifies the successful formation of crystallized TpTt-COF 30 .The corresponding peak shape is consistent with previous studies and simulated XRD.The chemical structure of COFs was analyzed by FTIR, as illustrated in Fig. 2b.The peak at 1620 cm −1 is attributed to the stretching vibration of the carbonyl group C=O in the β-ketoenamine moiety.The peaks at 1523 cm −1 and 1236 cm −1 correspond to the stretching vibrations of the C=C enamine carbon and the C-N bond at 1236 cm −1 , respectively.The peaks at 1384 cm −1 and around the other fingerprint regions originate from the monomers of Tp and Tt 36,41 , respectively, suggesting the formation of β-keto groups within the TpTt-COF.The XRD and FTIR data confirm the successful synthesis of TpTt-COF.Thermogravimetric analysis (TGA) was utilized to assess the thermal stability of COFs.As illustrated in Fig. 2c, a slight weight reduction was noticeable at low temperatures between 100 and 200 °C, likely due to the evaporation of water and residual organic solvents.When the temperature reaches 500 °C, the mass decreases significantly due to the total decomposition of TpTt.These observations imply that the COF structure is thermally stable under 200 °C.The Brunauer-Emmett-Teller (BET) method was used to analyze the specific surface area and pore structure of COFs. Figure 2d illustrates a type I isotherm with a BET specific surface area of 174.2 m 2 /g for the TpTt.This observation implies that TpTt-COF features a mesopore structure exceeding 10 nm in pore diameter, as shown from the BJH(Barrett-Joyner-Halenda) analysis in the inset in Fig. 2d.The pore structure agrees with the theoretical structure of TpTt-COFs.X-ray photoelectron spectroscopy (XPS) was employed to thoroughly examine the chemical composition of TpTt-COF.The XPS analysis, depicted in Fig. 2e, includes an XPS survey scan that distinctly illustrates the presence of carbon (C), nitrogen (N), and oxygen (O) elements within TpTt-COF.The N 1s XPS spectrum, presented in Fig. 2f, exhibits two prominent peaks corresponding to C-N and C=N in the triazine ring, with peak positions at 400.03 and 399.06 eV, respectively.In the O 1s XPS spectrum (Fig. 2g), the C-OH vibration peak of TpTt-COF is identified at 532.92 eV, while the C=O peak is observed at 531.32 eV.Simultaneously, the C 1s XPS spectrum (Fig. 2h) reveals three peaks at 284.8 eV, 286.52 eV, and 288.19 eV, corresponding to aromatic sp 2 hybridization C-C/C=C, C-N/C=N of triazine, and C=O of carboxylic acid.These findings, aligned with the specific figures, furnish essential details affirming the successful synthesis of TpTt-COF 42 , seamlessly connecting with PXRD and FTIR analyses.
The SEM morphology of the TpTt-COF sample is shown in Fig. 3a, b.TpTt-COF manifests as a crisscross fibrous structure with an average diameter of roughly 90 nm and an extending length of several micrometers.
The optical characteristics of COFs were investigated with UV-vis DRS.The inset in Fig. 4a shows the absorption spectrum of TpTt in the visible region with three peak maxima at 350, 420, and 525 nm.TpTt-COF offers a remarkably broad spectral response implying an extensive light-harvesting capacity, attributed to its extensive π-electron delocalization and the rapid occurrence of intramolecular charge transfer.The light absorption spectrum agrees with the dark orange color of TpTt shown in Fig. 2a, allowing its efficient absorption of a substantial portion of blue-green light, leading to a remarkably high efficiency in solar light utilization.Furthermore, the Tauc plot, as shown in Fig. 4a, was derived from the Kubelka-Munk equation with the bandgap energy of 2.62 eV for TpTt [43][44][45] , similar to the theoretical value of 2.657 eV 30 .

Photoelectrochemical analysis
Mott-Schottky analysis was employed to obtain the flat-band potential.As illustrated in Fig. 4b 4e, the band structure is presented.Figure 4f shows the Urbach tail analysis of the extinction coefficient, which is related to the density of defects [46][47][48] .Eu = 0.33 eV indicates mixed phases or some defects in TpTt.This particular characteristic is also evident in Fig. 4a, where a marginally smaller slope is observed in addition to the primary slope, affecting the Urbach tail with additional adsorption peak at 420nm 43,49 .
Transient photocurrent response was analyzed to investigate the photogenerated charge transfer.Referring to previous studies 50 , g-C 3 N 4 and TiO 2 were employed as conventional photocatalysts for a comparative analysis of the Photoelectrochemical properties and Photocatalytic activity of TpTt-COF.This approach enhances the objectivity of the experimental results.Figure 4c illustrates that TpTt-COF, g-C 3 N 4, and TiO 2 exhibited rapid on-off cycle photocurrent responses when exposed to visible light.This behavior is directly linked to the effectiveness of charge separation.Notably, the TpTt electrode displayed a distinctive initial spike in current 51 , which was insignificant for the g-C 3 N 4 and TiO 2 .We believe this is directly associated with the unique electronic structure of TpTt containing alternating adjacent electron donors and acceptors.When visible light irradiated the TpTt surface, photoexcited electrons were collected by the ITO and transferred to the counter electrode.Meanwhile, the excited holes were attracted to the electron donors (Tt) accumulated on the TpTt surface, leading to a positively charged surface.Subsequently, the accumulated holes will attract the photoexcited electrons on the (Tp) sites, initiating competition for electron migration.As a result, the photocurrent intensity decreased exponentially until the balance of surface charge density was achieved.Figure 4 reveals that g-C 3 N 4 exhibits the highest photocurrent, whereas TpTt experiences a substantially lower current intensity due to the charge trapping and recombination.However, introducing an appropriate amount of PMS significantly recovered the photocurrent intensity, while the initial peak current weakened considerably.This observation suggests that PMS can react with both the photoexcited electrons and holes directly on the surface of the TpTt.
EIS measurements were carried out to assess the charge transfer resistance at the electrode/electrolyte interface and examine charge transfer within COFs.As depicted in Fig. 4d, the semicircle diameter of the Nyquist plot from the TpTt-COF is markedly smaller than that from g-C 3 N 4 and TiO 2 , indicating a lower charge transfer resistance, possibly due to the presence of both electron donor and acceptor at the adjacent part of the TpTt molecule.

Photocatalytic activity and mechanism
To evaluate the photocatalytic efficacy of TpTt-COF in conjunction with PMS, dye degradation kinetics measurements were carried out for solutions containing 10 mg/L of RhB, MB, and MO, as illustrated in Fig. 5a.While TpTt-COF demonstrated the highest adsorption capacity for MB during the initial adsorption process in the dark, the subsequent photocatalytic process revealed that RhB exhibited the highest photodegradation rate.Hence, RhB was selected as an example for further investigation into TpTt-COF's performance in degrading dyes.
Figure 5b shows that PMS alone exhibited a low degradation rate in both dark and illuminated conditions with the rate constants of 0.655 min −1 and 2.234 min −1 , respectively.For the TpTt without PMS, a degradation rate constant of 5.502 min −1 was achieved.However, with TpTt combined with PMS, it was increased to 8.856 min −1 , 1.6 times that of TpTt alone or 4.0 times that of PMS alone.Hence, the fast degradation kinetics can only be achieved with the synergistic effects of TpTt and PMS.In comparison, from Fig. 5c, the degradation rate constants for g-C 3 N 4 and P 25 (TiO 2 ) combined with PMS are 0.636 min −1 and 0.732 min −1 , respectively.However, without PMS, the corresponding K values decrease to 0.146 min −1 and 0.112 min −1 , respectively.Thus, TpTt offers much better photocatalytic performance through the activation of PMS in comparison with traditional or commercial photocatalysts, such as g-C 3 N 4 and P 25 (TiO 2 ).This is because TpTt can supply both photoexcited electrons and holes to facilitate the activation of PMS and generation of •O 2 -and •SO 4 -radicals.For traditional n-type photocatalysts, normally only excited holes are responsible for producing oxidative radicals, and the photoexcited electrons are consumed by producing hydrogen on the counter electrode in an aquatic environment.Figure 5d illustrates that the TpTt's photocatalytic performance gradually improves as the pH decreases.This improvement may be attributed to the nature of surface functional groups on the catalyst 52 , which might affect the balance between the trapped photoexcited electrons and holes.
To investigate the synergistic mechanism for the photocatalytic degradation of dyes using TpTt-COF enhanced with PMS, different radical scavengers, including IPA, BQ, EDTA, and MeOH, were added to quench •OH, •O 2 − , h + , and •SO 4 − , respectively.Figure 6a shows that the addition of IPA, EDTA, and MeOH had similar minor inhibitory effects, indicating that •OH, h + , and •SO 4 − play less important roles in the degradation of RhB.However, introducing an appropriate amount of BQ exhibited the strongest inhibitory effect by decreasing the rate constant by 87%, indicating that •O 2 − is the dominant active radical.The result is summarized in Fig. 6b.Furthermore, Fig. 6c  The excitation process is proposed here.When light illuminates the surface of TpTt, it initiates process (Eq. 1) to produce excited electrons and holes.The reaction of electrons with O 2 produces the •O 2 − (Eq.2), which can recombine with hole (Eq.3), causing a rapid decline in photocurrent intensity and the appearance of the initial (1) www.nature.com/scientificreports/quenched by IPA (Fig. 6b).Meanwhile, the SO 5 − will also react with H 2 O, producing the reactive •O 2 − radical (Eq.7) 56 .Hence, two possible pathways exist for producing the •O 2 − radicals through either the direct reduction of O 2 by photoexcited electrons on TpTt (Eq.2) or the oxidation of H 2 O mediated by activated PMS (Eqs.6 and 7).Nonetheless, adding PMS will utilize both photoexcited electrons and holes in the degradation of RhB with a synergistic effect.Figure 6d confirms that an increase in the quantity of TpTt substantially accelerated the degrading kinetics since more PMS can be activated to produce •O 2 − radicals.PMS is gradually consumed in this process since the increase in the RhB concentration confirmed the limited degradation capacity in Fig. 6e, although the initial degradation rate was maintained.After PMS was depleted, the degradation rate was significantly reduced, represented by the declining rate constant, as shown in Fig. 6f.

Reusability and stability
The reusability and performance stability are critical factors in assessing the commercial viability of a photocatalyst.As illustrated in Fig. 7a, even after five cycles of photocatalysis, TpTt continues to exhibit an impressive efficiency of 83.2% for RhB degradation.The XRD spectrum in Fig. 7b shows there is minimal change in the structural integrity 57,58 .Hence, the synthesized TpTt, as a reusable, efficient photocatalyst, holds considerable promise for practical applications.
The reaction and process illustrated in Equations (1-7) are also shown in Fig. 8. Without PMS, the excitation process for the TpTt is proposed as Fig. 8a, aligning with the general mechanism of photocatalysis.When TpTt-COF is excited by visible light, electrons (e − ) and holes (h + ) are generated.Electrons react with oxygen in the water environment to produce •O 2 − , while holes react with OH − in water to generate •OH.Of course, electrons and holes also rapidly react, representing the fast recombination of holes and electrons in TpTt-COF.The descriptions of the mechanisms mentioned above, in which TpTt is combined with PMS, can all be visually demonstrated in Fig. 8b.In the process of TpTt-COF binding with PMS, it not only reacts with electrons to produce SO .This process not only promotes the generation of various free radicals but also facilitates the effective separation of electrons and holes, significantly reducing the recombination of electrons and holes, presenting an intriguing synergistic effect.Of course, in the case of combining with PMS, reactions conforming to the fundamental photocatalysis rules also occur, where electrons and holes react with •O 2 − and •OH produced by oxygen in the water environment and OH − in water, respectively.The generated free radicals, including holes themselves, actively participate in the degradation process of pollutants, breaking them down into small molecular intermediates, and even into carbon dioxide and water.

Conclusions
This study achieves innovative degradation of organic dyes under visible light by exploring the combined application of TpTt-COF and PMS.The synthesized orange TpTt-COF monomer demonstrates outstanding photocatalytic properties, environmental adaptability, and sustainability, positioning itself as a potential candidate for the photocatalytic degradation of organic dyes in water environments.The study effectively addresses the challenge of high charge recombination in TpTt-COF monomers.In comparison to traditional photocatalytic materials, the degradation rate of TpTt-COF combined with PMS is 13.9 times higher than PMS combined with g-C 3 N 4 and 1.

Figure 1 .
Figure 1.Schematic diagram of the preparation process for TpTt-COF photocatalyst.

Figure 2 .
Figure 2. (a) The measured and simulated XRD patterns, (b) FTIR spectrum, (c) TGA data, (d) N 2 adsorptiondesorption isotherms of TpTt-COF, the inset in (a) shows the color photograph of the sample, and the inset in (d) is the pore diameter distribution from the BJH analysis.(e) XPS spectrum of TpTt-COF.High-resolution XPS spectra of (f) N 1s, (g) O 1s, (h) C 1s of TpTt-COF.
, TpTt-COF exhibits positive slopes in the Mott-Schottky plot, indicating an n-type semiconductor.The flat-band potential (E fb ) of TpTt-COF was −0.96 V vs Ag/AgCl.It's widely recognized that the flat-band potential of an n-type semiconductor is close to its conduction band (CB) potential.Hence, the E CB of TpTt is approximately −1.16 V vs. normal hydrogen electrode (NHE).From the band gap energy of 2.62 eV, the valence band (VB) potential of TpTt-COF is 1.46 V vs. NHE.Figure 4e presents the XPS spectrum showing the valence band edge of TpTt at 1.70 V with the instrument's work function (E function ) of 4.2 eV.It can be obtained by the formula 43 (E VB,NHE = E function + E VB,XPS − 4.44 ) This concurs with the previously inferred valence band value of TpTt, resting at 1.46 V.In the inset in Fig.
reveals that the K value increases with increasing PMS mass, reaching a maximum value with 25 mg of PMS.Hence, excess PMS can lead to the generation of •OH and •SO 4 -, reducing the concentration of •O 2 − with decreased performance.

Figure 5 . 2 Figure 6 .
Figure 5. (a) The concentration evolution during the photocatalytic degradation of RhB, MO, and MB dyes with PMS and TpTt-COF at pH3, (b) RhB degradation with PMS, TpTt, and their combination in dark and visible light excitation, (c) g-C 3 N 4 and P 25 (TiO 2 ) control group, (d) photocatalytic RhB degradation rate constant as a function of pH.